FINITE ELEMENT ANALYSIS OF TI-6AL-4V
ELI AND ZIRCONIA BIO-INERT MATERIAL
USED IN MOLAR TOOTH DENTAL IMPLANT
Sharanraj. V1 and Dr. C.M. Ramesha2
Biomaterial is a non-viable material used in the field of medical dental implantation, which is intended to interact
with biological system. A dental implant is an artificial substitute for the replacement of missed tooth. Based on the
biological interaction with material, biomaterials are categorized into three types. i.e., Bio-inert materials, Bio-active
materials and Bio-resorbable materials. Bio-inert materials are those materials which has minimum interaction with
the surrounding tissue namely Titanium alloy (Ti-6AL-4V ELI) and Zirconia . Bio-active materials are those
materials when placed in a human body interact with the surrounding tissues namely glass, ceramics and Bioglass.
Bio-Resorbable materials are those materials which start dissolving when placed in human body and slowly replaced
by the advancing tissue namely bone. But today Bio-inert materials have been extensively used in dental implants,
due to their unique characteristics like good biocompatibility, high yield strength and high corrosion resistance .
Dental Anatomy is a field of anatomy dedicated to the study of tooth structure and as shown in Fig.1. A dental
1 Department of Mechanical Engineering M.S. Ramaiah Institute of Technology, VTU, Bangalore - 560054, Karnataka, India
2 Department of Mechanical Engineering M.S. Ramaiah Institute of Technology, VTU, Bangalore - 560054, Karnataka, India
International Journal of Latest Trends in Engineering and Technology
Vol.(8)Issue(1), pp. 264-271
Abstract- Ti-6AL-4V ELI and Zirconia are the important bio-inert materials used in the field of dental implant due to their
unique characteristics of minimal interaction with surrounding tissue. This paper presents the typical Finite element method
(FEM) is an effective approach for analysis of dental implant and dental structures. In the present work, 3 dimensional
modeling of molar tooth was generated by CATIA V5 software and analysis were carriedout by commercial FEA software
Ansys 14.5 to evaluate the displacement, strain, stress, fatigue life and factor of safety in the proximal region of Ti-6Al-4V
ELI and Zirconia molar tooth implant under static load condition of 50, 100, 150, 200, 250 and 300 newton. The results
show that the displacement, strain and stresses, fatigue life and factor of safety were within the material admissible limits for
Zirconia. Hence the study reveals that Zirconia is an alternate biomaterial suitable for dental implants.
Keywords – Bio-inert material, Ti-6Al-4V ELI, Zirconia, FEM.
Finite Element Analysis Of Ti-6al-4v Eli And Zirconia Bio-Inert Material Used In Molar
Tooth Dental Implant Application 265
Fig.1. Dental Anatomy (a) Molar tooth location (b) Molar tooth structure .
implant is an artificial substitute for the root of a tooth that is placed into the jawbone, and ultimately fuses with the
bone in order to support a replacement tooth. The teeth are the hardest substances in the human body. Besides being
essential for chewing, the teeth play an important role in speech . After a tooth has been damaged or decayed,
restoration of the missing structure can be achieved with a variety of treatments from variety of materials, including
Titanium alloy (Ti-6Al-4V ELI) and Zirconia are small restorations placed inside a tooth are referred to as
These restorations may be formed directly in the mouth or may be cast using the lost-wax technique, such as for
some inlays and onlays. When larger portions of a tooth are lost, an extracoronal restoration may be fabricated, such
as a crown and screw or implant, to restore the decayed tooth. A normal adult mouth has 32 teeth, which have
erupted around age 18. Parts of the teeth include: Enamel, Dentin, Pulp Cavity, Crown, Root, Cement, Gum Tissue,
Incisors, Canines, Premolars and Molars . Molar are flat tooth located at rear end of the mouth for the best
grinding of food and the only tooth which can withstand maximum load upto 300N. Hence 3D modeling and Finite
element analysis is carriedout on molar tooth by applying Ti-6AL-4V ELI and Zirconia material properties in the
As in . Author has aimed the study to provide a detailed description of crown-size dimension in the
deciduous dentition of people and to compare the findings with those of other populations. Measurement of
mesiodistal (MD) and buccolingual (BL) crown diameters were obtained from dental casts of 84 males and females
aged 2.9 years to 18 years. The differences in crown size (MD and BL diameters) between the right and left sides of
the dental arch were not significant.Ti-6Al-4V ELI composition consists of Ti 89% wt, Al 6% wt and V 4% and is
widely used for implants and other porous surface-coating and contains impurities (N, 0.13% O, Fe, H and C). Extra
Low Interstitials (ELI) includes impurities increasing interstitial content that increase strength and fatigue limit. (N
increases hardness, O increases tensile strength), but has unsatisfactory wear.
Ti-6Al-4V ELI having yield strength 114 GPa is widely used in dental implants due to their unique
characteristics such as lower modulus, superior tissue compatibility and high corrosion resistance. But then the
presence of vanadium in Ti-6Al-4V ELI alloy will cause long health related problems . Hence it is no longer the
case that titanium is considered as completely bio-inert material. In contrast, titanium is thought to be the” New
Allergen” as demonstrated by several reports and studies . Titanium has entirely replaced other metals in dental
implants. Titanium is also widely used in oral and maxillofacial surgery to form other devices such as grids,
membranes, plates, screws and tooth. The mechanical properties can be enhanced when titanium is alloyed, but
sometimes deteriorates the corrosion resistance properties and constituent release can be substantially reduced with
surface treatments of titanium or its alloy. The author concluded that titanium release from the devices stops only
after bone is laid down on the titanium surfaces and titanium release does not seem to interfere with the osteogenic
process but perhaps may interact with it .
Zirconia (ZrO2) ceramics have superior mechanical properties for biomedical applications compared to other
ceramics, exemplified by higher fracture toughness, higher flexural strength, and lower Young’s modulus 205
GPa (giga pascal). There are two types of zirconia ceramics commonly used for surgical implants: yttria-
stabilized tetragonal zirconia and magnesium oxide partially-stabilized zirconia . Partially stabilized
zirconia is practically used today in manufacturing of dental crown. As in  author has a focus of interest in
implant dentistry in the application of ceramic materials for the fabrication of implant abutments as well as for
dental implants. When compared to Zirconia ceramic, the enhanced strength of zirconia was explained by
microstructural differences such as higher density, smaller particle size and had performed FEM analyses of sound
and restored teeth to evaluate stress distribution assessment. This method is efficient approach to mechanical and
fracture behavior of systems with complex geometry and with materials with different mechanical properties
submitted to different loading modes .
FEM analysis is a powerful tool to characterize dental systems in their different functional conditions, being of
great importance to both dentists and engineers . In vitro tests of sound and restored teeth are being submitted to a
static and cyclic loading under functional conditions by biomaterials group to validate the numerical results obtained
from FEM. As in  author has investigated the biomechanical behavior of a threaded functionally graded
biomaterials dental implant surrounding bone system under static and harmonic forces by using a three-dimensional
finite element method. The interaction of the implant and the supporting bone tissues is considered. Three contact
conditions at the implant–bone interface are used to model different osseointegration stages. A comprehensive
parametric study was conducted to highlight the influence of the material properties and the osseointegration quality
on the maximum von-Mises stress, deformation distribution and natural frequencies.
Sharanraj. V and Dr. C.M. Ramesha 266
II. FINITE ELEMENT AND EXPERIMENTAL PROCEDURE
A. Geometric Modeling
The first step in FEM is a geometric modeling . In this step the three dimension (3D) model of molar tooth with
implant is generated by using CATIA V5 software is illustrated in Fig. 2(a) and 3D model is converted into step file
format (STP) shown in Fig. 2(b).
Fig. 2(a) 3D model of molar tooth with implant in CATIA, (b) 3D model converted into STP.
Geometrical dimension of molar tooth are validated against actual tooth and implant by measuring key dimension
listed in Table 1.
Table 1: Comparison of key dimension of tooth
Molar tooth with implant
by CATIA V5
Height of Crown (mm) 07 07
Perimeter of Crown at middle (mm) 24 24.015
Height of implant (mm) 10 10
Perimeter of Implant (mm) 15.5 15.71